In Vitro Evaluation of Shear Bond Strength of Nanocomposites to Dentin
Swati Gupta1, Vinay Kumar Vellanki2, Vikram Shetty K3, Sudhanshu Kushwah4, Geeta Goyal5, S.M. Sharath Chandra6
ABSTRACT Aims: To compare the shear bond strength of nanocomposites to dentin using three different types of adhesive systems; and to test few specimens under Scanning Electron Microscope (SEM) for analysing whether the bond failure is adhesive or cohesive. Materials and Methods: Sixty human premolar teeth were selected and were randomly grouped, with 20 specimens in each group: group 1 - fluoride releasing dentin bonding agent; group 2 - antibacterial containing dentin bonding agent; and group 3 - one step conventional self etch adhesive. Each group was treated with its respective bonding agents, composite resin build up was done, and shear bond strengths were tested using Instron Universal testing machine. Few of the specimens were tested under SEM.
Results: The results were statistically analysed using Oneway ANOVA and paired t-test. It was observed that group 3 has the highest shear bond strength followed by group 2, and then group 1. Adhesive failures and mixed failures were most frequent types of failures as seen under SEM. Conclusion: Addition of antimicrobial agent decreases the bond strength of dentin bonding agent and addition of fluoride further decreases the bond strength. From SEM results it can be concluded that the zone of failure could not be defined and also that the failure mode was independent of the dentin bonding agent used.
Keywords: Antibacterial, Dentin bonding agents, Fluorides, Nanocomposites, Self etch adhesives, Shear bond strength, Total etch adhesives
Introduction Adhesive dentistry is a rapidly evolving discipline. For many years, the dental profession has strived to achieve good adhesion of resin composite to tooth substrate . In 1955, Bunocore introduced the concept of acid etching of the enamel which later on gave way to total etch techniques . The total etch adhesives provide good bond strength yet newer concepts of self etching system have been developed and have proven to be good clinically . Self etching primers combine both dentin conditioning and bonding in a single step . The introduction of antibacterial properties into the bonding agents is a new concept. For dentin bonding agents, either fluoride can be incorporated in them , or monomers by themselves may produce antibacterial effects. Methacryloxydodecylpyridiniumbromide (MDPB), a new monomer, shows antibacterial activity against bacterial growth and plaque accumulation . The replacement of composite resin restorations due to secondary caries at restoration-tooth interface is still one of the greatest problems . The decreased incidence of secondary caries along the margins of silicate restorations led to the development of fluoride releasing composite resins . However, the bonding agent applied prior to the placement of resin may bock the passing of fluoride to the exposed dentin. This led to the introduction of fluoridated bonding agents . Thus, with this background, the present study was undertaken to compare the shear bond strength of nanocomposites to dentin using fluoride releasing 7th generation dentin bonding agent, antibacterial (MDPB) containing dentin bonding agent, and conventional one step self etch system; to test whether these additional agents have any effect on the shear bond strength of these adhesives; and to test some of the specimens under Scanning Electron Microscope (SEM) for analysing whether the bond failure is adhesive or cohesive. The present study assesses the shear bond strength as it has been Journal of Clinical and Diagnostic Research. 2015 Jan, Vol-9(1): ZC09-ZC11
proven to be useful as a screening tool to help understand and predict the clinical behaviour of adhesives .
Materials and Methods The study was conducted in the Department of Conservative Dentistry and Endodontics, Krishnadevaraya College of Dental Sciences & Hospital, Bangalore, Karnataka, India. The study was started in August 2012 and was conducted over a time period of eight months. The institutional ethical committee approved this study. Study sample, inclusion and exclusion criteria: Sixty freshly extracted human pre-molars were collected. Teeth extracted within six month period were included as study sample. Teeth with caries, fracture or cracks, teeth with anatomical variations, teeth with pre existing restorations, and teeth affected with flourosis were not included in the present study. Preparation and grouping of the specimens for shear bond strength: Based on the dentin bonding agent used teeth were divided into three groups of 20 teeth each: group 1 - fluoride releasing 7th generation dentin bonding agent (Bond Force Tokuyama Dental Corp); group 2 - antibacterial (MDPB) containing dentin bonding agent (Clearfil Protect Bond- Kuraray); and group 3 - one step conventional self etch adhesive (Xeno-V Dentsply). Teeth were mounted in stainless steel holders with the help of self cure acrylic resin (DPI) to embed the root portion. These stainless steel holders were colour coded according to the groups i.e. red colour for group 1, yellow colour for group 2, and green colour for group 3. The occlusal surfaces of teeth were grounded with the help of a diamond disk (DFS Germany) mounted on a straight micromotor hand piece (NSK Japan) to prepare flat surfaces at a depth of 1.5 mm from the cuspal tip of the tooth. Bonding agents were applied to all the specimens as per manufacturer’s instructions and then light cured accordingly. Filtek Z350 XT (3M ESPE) composite was 9
Swati Gupta et al., Shear Bond Strength Nanocomposites to Dentin N